DAMAGE MECHANICS MODELING OF CONCURRENT THERMAL AND VIBRATION LOADING ON ELECTRONICS PACKAGING


 Coleen Dixon
 2 years ago
 Views:
Transcription
1 Multidiscipline Modeling in Mat. and Str., Vol. 2, No.3, pp (2006) BRILL Also available onlinewww.vsppub.com DAMAGE MECHANICS MODELING OF CONCURRENT THERMAL AND VIBRATION LOADING ON ELECTRONICS PACKAGING Juan Gomez 1, Minghui Lin 1 and Cemal Basaran 2 1 Research Assistant, UB Electronic Packaging Laboratory. 2 Professor, and Director, UB Electronic Packaging Laboratory University at Buffalo, State University of New York Received 3 February 2005; accepted 26 October 2005 Abstract The problem of concurrent thermal and vibration loading has not been thoroughly studied even though it is common in electronic packaging applications. Here we attempt to address such a problem using a damage mechanics based constitutive model. Damage mechanics constitutive model for eutectic Pb/Sn solder alloys is used to simulate the damage effects of concurrent cyclic thermal loads and vibrations on Ball Grid Array (BGA) packages. The model is implemented into the commercial finite element code ABAQUS through its user defined material subroutine capability. For the integration algorithm we have used a return mapping scheme, which dramatically improves the convergency rate as compared to previous implementations of the same model. Results are examined in terms of accumulation of plastic strain within the solder connections. It is shown that the simplistic Miner s rule can not accurately account for the combined effect of both loadings acting concurrently. Keywords: Finite element analysis, constitutive model, dynamic analysis, concurrent loading, microelectronics packaging, solder joints. 1. INTRODUCTION The most common mode of failure in microelectronic packaging solder joints is low cycle fatigue. Temperature changes and the coefficient of thermal expansion mismatch between the soldered parts is the main reason behind the fatigue. When an electronic package undergoes a temperature variation interconnects are stressed mainly in cyclic shear. The stresses impart elastic and inelastic strains, which are also cyclic in nature leading to thermo mechanical fatigue. The temperatures changes are due to switch on/off operations or sometimes owing to fluctuations in the ambient conditions. On the other hand, eutectic solder alloys are routinely used at high homologous temperatures. The melting point of the eutectic Sn/Pb solder alloy is 183 C, and it is at 0.65T m at room temperature, where T m is the melting point. Therefore, solder joints exhibit time, temperature, stress dependent deformation behavior and such coupling makes constitutive modeling a difficult task. Material models ranging from purely elastic to elastoviscoplastic using various stressstrain relations have been proposed for Sn/Pb
2 310 Juan Gomez, Minghui Lin and Cemal Basaran solder alloys, such as in Kitano et al.(1988),[1], Lau & Rice(1990),[2], Basaran et al.(1998),[3] and many others. Adams (1986), [4] proposed a simple viscoplastic model without hardening. Wilcox et al (1989), [5], proposed a rheological model to represent the inelastic behavior of the material, however it is applicable to a limited range of strain rates. The purely phenomenological models proposed by Knocht and Fox (1990), [6], Darveaux and Banerji (1992), [7] and Hong and Burrell (1995), [8] decoupled the creep and plasticity effects artificially. This decoupling does not have any physical basis and is just motivated by mathematical convenience. Classical forms of decoupled plasticity and creep theories have been shown to be quite inferior for modeling cyclic plasticity, creep and interaction effects, Mcdowell et al(1994),[9]. Recently, Zhao(2000),[10], followed by Basaran and Tang (2002), [11] and Tang (2002), [12] have extended a creep law originally proposed by Kashyap and Murty(1998), [13] for eutectic solder alloys into a thermodynamics based framework for low cycle fatigue predictions. The model has been validated against thermomechanical fatigue experiments, Gomez and Basaran, (2005a), [14], performed on thin layer solder joints and nanoindentation experiments at room temperature, Gomez and Basaran (2005b), [15]. Another source of failure in electronic equipment is vibrations, Steinberg (2000), [16]. It is common for electronic equipment to be subjected to vibrations over a wide range of frequencies and acceleration levels. For instance, according to the US Air Force, vibration and shock loads are responsible for the mechanical failure of 20 percent of airborne electronics. These vibrations may occur simultaneously with thermal loads at some time during the service life of the structure. However, this combined effect has not been thoroughly studied or understood by the electronic packaging community, Basaran et al (2001), [17]. This is in part because of the lack of robust constitutive models to predict the creepvibrationfatigue interaction effects on eutectic solder alloys. Also the vibration and thermal cycling effects occur at different time scales which make the computational treatment highly expensive. On the other hand, there is not enough experimental data for verification of the computational models. In this paper we have implemented a constitutive model into the commercial finite element code ABAQUS through its user defined material subroutine capabilities. We have used a return mapping scheme as proposed in Simo and Hughes (1997), [18]. Previous ABAQUS implementations of similar models like in Tang(2002), [12], Basaran and Tang (2002), [11], Basaran et al(2005),[17] have made use of the Owen and Hinton(1980),[19] viscoplasticity integration scheme which when ported into ABAQUS exhibits very low convergence rate making it impractical if not impossible for dynamic loading applications. The main goal of the present paper is to study the combined effect of dynamic loads applied concurrently with thermal cycling. Although we do not directly calculate the fatigue life in our simulations, conclusions about the fatigue life are inferred from the computed inelastic strains and damage parameter under combined conditions. Experimentally, this problem was addressed by Zhao et al (1999), [20] where concurrent vibration and thermal cycling was performed on a commercial electronic package using a dynamic shaker embedded into a controlled thermal chamber. The effect on fatigue life of the concurrent loading conditions was described in terms of the plastic strains measured by high sensitivity Moire interferometer technique. Based on the boundary conditions, and loading profile they used it was concluded that the fatigue life is improved when the loads are applied concurrently and that the commonly used Miner s rule to superimpose the effects of the two loads acting independently is inaccurate. According to Barker et al (1990), [21],
3 Damage Mechanics Modeling of Concurrent Thermal. 311 Miner s rule, Miner (1945), [22] assumes that every structural member has a useful fatigue life and that every stress cycle uses up a part of this life. Furthermore, if the strains from vibrational and thermal loading are available, Miner s rule assumes that the nth nv fatigue life can be characterized like R = + where R is the ratio of number of N th N v cycles experienced n i to the fatigue life N i at a specific i th strain level. The fatigue life at a given strain level is commonly computed using CoffinManson relations or modified CoffinManson relations which was developed for structural steel. Miner s rule is intended as a first order approximation since it can not account for factors like creep and the temperature dependent dynamic properties of the structure. For instance, as the thermal load progresses certain parts of the package may soften or harden, leading also to changes in the natural frequencies of the structure and therefore to its dynamic response. However, we inhere show that even if the superposition trend of the Miner s rule is correct, it may not yield accurate results quantitatively when predicting fatigue life because it does not account for nonlinearities that may occur during the loading process. Moreover, we show here that Miner s rule may lead to nonconservative results. In order to prove our point we have conducted two sets of finite element analysis. First, we model a commercial personal computer PCB with all the mounted components where we conduct several analyses to show that the trend behind Miners rule is correct. Then we model a microprocessor package where we conduct several analyses to show that the trend behind Miner s rule is correct qualitatively. In this work we assume that the equivalent plastic strain reveals the damage trend even if it may not be quantitatively very accurate, Basaran et al (2005), [17]. 2. MATERIAL CONSTITUTIVE MODEL In the implemented constitutive model the return mapping scheme is the one after Simo and Hughes (1998), [18] and Lubarda and Benson (2002), [23] viscoplastic integration and the Alfano et al (2001), [24] scheme for the nonlinear kinematic hardening model are used. Damage is introduced using the effective stress concept and the strain equivalence principle. Rate dependent effects are considered by means of the viscous overstress concept. Here we present the flow theory formulation following the classical approach in terms of a yield function separating the elastic from the viscoplastic domain, a flow rule specifying the evolution of the viscoplastic strain, a set of hardening laws specifying the evolution of the hardening parameters and the evolution of damage like an additional state variable. In order to describe the model it is convenient to first present the equations for a rate independent material without any damage Hooke s Law For a classical Von Mises rate independent plasticity model with isotropic behavior Hooke s law reads p θ & σ = C & ε & ε & ε (1) : ( )
4 312 Juan Gomez, Minghui Lin and Cemal Basaran p where & ε, & ε and θ ε& are the rates of total strain, plastic strain and thermal strain respectively, C is the elastic constitutive tensor and : represents contraction between two tensors Yield surface The elastoplastic domain is defined according to the following yield function 2 F = S X K( α ) S X R( α) (2) 3 where F( σ, α ) is a yield surface separating the elastic from the inelastic domain, X is the deviatoric component of the back stress describing the position of the center of the yield surface in stress space, S is the deviatoric component of the stress tensor, 2 A A A represents the norm of a given tensor A, R( α ) K( α ) describes 3 the radius of the yield surface in stress space Flow rule The evolution of the plastic strain is represented by the general flow rule, P & ε = γ nˆ (3) F with nˆ = being the normal to the yield surface. σ 2.4. Isotropic hardening Isotropic hardening is described by the evolution of the radius of the yield surface according to 2 c K( α ) = Y0 + R ( 1 e α ) (4a) 3 where α is a plastic consistency parameter or plastic strain trajectory evolving according to (4b), Y 0 is the initial yield stress, R is an isotropic hardening saturation value and c is an isotropic hardening rate. 2 & α = γ (4b) The NonLinearKinematic Hardening (NLK) Rule The NLK rule is taken from Chaboche (1989), [25] and was originally proposed by Armstrong and Frederic (1966),[26]. Nonlinearities are introduced as a recall term to the Prager (1956), [27] linear rule. p X & = c & ε c X & α (5) 1 2
5 Damage Mechanics Modeling of Concurrent Thermal. 313 The first term represents the linear kinematic hardening as defined by Prager. The second term is a recall term, often called a dynamic recovery term, which introduces the nonlinearity between the back stress X and the actual plastic strain. When c 2 = 0 Eqn. (5) reduces to the linear kinematic rule. The NLK equation describes the rapid changes due to the plastic flow during cyclic loadings and plays an important role even under stabilized conditions (after saturation of cyclic hardening). In other words, these equations take into account the transient hardening effects in each stressstrain loop. After unloading, dislocation remobilization is implicitly described due to the back stress effect and the larger plastic modulus at the beginning of the reverse plastic flow Chaboche (1989), [25]. Note than in equation (5) c 1 corresponds to the term 2 C in the 3 original formulation and described in Basaran et al (2005), [17]. In the equations above, γ is a nonnegative plasticity (consistency) parameter representing the irreversible character of plastic flow and obeying the following properties. 1. For a rate independent material model γ obeys the socalled loading/unloading and consistency condition γ 0 and F( σ, α) 0 (6) γf( & σ, α ) = 0 (7) 2. For a rate dependent material model conditions (6) and (7) are replaced by a constitutive equation of the form. φ( F) γ = (8) η where η represents a viscosity material parameter. In the case of a rate independent material F satisfies conditions (6) and (7) and additionally stress states such F( σ, α ) > 0 are ruled out. In the case of a rate dependent material on the other hand, the magnitude of the viscoplastic flow is proportional to the distance of the stress state to the surface defined by F( σ, α ) = 0. Using this fact we have after using Eqn.(8) that the following relation can be established F =Θ ( γη ) (9) 1 Θ γη = φ γη. where ( ) ( ) 2.6. Viscoplastic creep law In this particular model the creep law is the one proposed by Kashyap and Murty (1981), [12] and extended to multiaxial case by Basaran and Tang (2002), [11] and given by n p vp AD0 Eb F b Q / Rθ F & εij = e (10) kθ E d σ ij where, A is a dimensionless material parameter which is temperature and rate dependent,
6 314 Juan Gomez, Minghui Lin and Cemal Basaran D Q/ Rθ i = D0e is a diffusion coefficient with 0 D representing a frequency factor, Q is the creep activation energy, R is the universal gas constant, θ is the absolute temperature in Kelvin, E( θ ) is a temperature dependent Young s modulus, b is the characteristic length of crystal dislocation (magnitude of Burger s vector), k is Boltzman s constant, d is the average grain size, p is a grain size exponent, n is a stress exponent for plastic deformation rate, where 1/n indicates strain sensitivity. p n kθ d Q/ Rθ From Eqn.(10) we can identify φ ( F) = F and η = e n 1. AD E b b 2.7. Damage coupled elastoviscoplastic model Making use of the strain equivalence principle we can write in the usual form, Lemaitre (1996), [28] vp θ & σ = 1 DC:( & ε & ε & ε ) (11) ( ) F = D 2 D S X ( 1 D) K( α ) S X 3 ( 1 D) R( α) (12) where D is a damage metric and D X = 1 D vp c ε c X α (13) 2.8. Formulation of damage function ( )( 1 2 ) Damage is considered following the approach by Basaran and Yan (1998), [29], Tang (2002), [12], Basaran and Nie (2004), [30], where the relation between the disorder and entropy established by Boltzmann using statistical mechanics and the second law of thermodynamics is exploited. Their thermodynamic framework assumes that damage and the disorder are analogous concepts and the thermodynamic disorder can be used to model the damage evolution. The damage formulation used here has the advantage over other damage formulations that is not derived from a damage potential and therefore there are not additional material properties. Thus, damage can be completely characterized using standard material properties. The Damage evolution function is given by D = 1 e (( e φ) /( N0kθ / ms )) D cr (14) where D cr is a damage threshold e φ is the difference between the changes in the internal energy and the Helmholtz free energy with respect to a reference state. This difference is obtained as follows: the internal energy equation, which is an expression of the first law of thermodynamics, reads de in ρ = σ ˆ ijdij + ργ qi, i (15) dt 0
7 Damage Mechanics Modeling of Concurrent Thermal. 315 in where D ij is the rate of deformation tensor. For the particular case of small strains and in dε in ij small displacements Dij =. ˆ γ is the internal heat production rate and q i is the dt rate of heat flux through the surface. The Helmholtz free energy is written in terms of the stress tensor thus dψ in ρ = σijdij (16) dt After combining Eqs. (15) and (16), the difference between the changes in the internal energy and the Helmholtz free energy with respect to a reference state is obtained as follows; t2 t2 t2 S in ij ij i, i t1 t1 t1 1 e φ = σ D dt + γdt q dt ρ (17) This damage evolution model and integration algorithm has been verified against nanoindentation and fatigue experiments performed at the UB electronic packaging lab under different temperatures and imposed displacement rate conditions, Basaran and Yan (1998), [29], Basaran and Tang (2002), [11], Gomez and Basaran (2003), [31]. 3. FINITE ELEMENT SIMULATION OF CONCURRENT LOADING ON A PRINTED CIRCUIT BOARD In order to study the response under concurrent thermal and vibration loads using the constitutive model described above we have modeled an actual electronic package using the commercial finite element code ABAQUS where the constitutive model has been implemented by a user subroutine UMAT.. The studied assembly consists of a personal computer Printed Circuit Board (PCB) with the most relevant components mounted. The PCB is approximately 305mm long x 270mm wide with a thickness of 1.6mm and made of epoxy fiberglass known as FR4. Properties for the materials other than solder joints are obtained from Pecht et al (1999), [32] and reported in Table 1. Pitarresi (2001), [33] performed dynamic testing and linear elastic finite element simulations of a similar PCB considering all the attached components. However the author did not consider the solder joints. In that study the natural frequencies and modal shapes of the PCB were measured and calculated with a 3D finite element model and the average stiffness and effective Young s modulus for different parts of the structure were measured. From the Pitarresi (2001), [33] analysis it is apparent that the fundamental mode of the structure induces flexure at the chipset and the processor locations. This is consistent with damage observed in the BGA solder joints during transportation. The corresponding finite element mesh is shown in Figure 1. In the first analysis set, we applied dynamic loading with amplitudes representative of those typically encountered during the service life, at 3 different frequencies and under isothermal conditions at room temperature. The dynamic loading was applied in the horizontal direction by imposing an acceleration history at the supported ends. A schematic of the applied dynamic load is shown in Figure 2. Second, we applied thermal loads only with the profile shown in Figure 3. In the final set of
8 316 Juan Gomez, Minghui Lin and Cemal Basaran analyses we applied the dynamic and thermal loads concurrently. The package was fully fixed at the ends, and the dynamic loading in form of input acceleration was prescribed at the support points and in the vertical direction. Modal analysis was performed first to determine the natural dynamic properties of the package. The first 5 modes are presented in Figure 4. Table 2 shows the first five natural frequencies of the structure. For the dynamical response an implicit direct integration scheme was used. The applied loads were harmonics with frequencies of 1Hz, 45Hz and 100Hz. Tab.1 Material properties for the elastic components Material E (GPa) σ y (MPa) ν ρ (tonne/mm^3) Pb37/Sn E09 BT E09 FR E09 UL 94V E09 Tab.2 Free vibration frequencies for the structure Mode Frequency(Hz) unloaded (a) (b)
9 Damage Mechanics Modeling of Concurrent Thermal. 317 Fig.1 (a) Complete Finite Element Model. (b) Mesh at the chipsetpcb region. Dynamic Loading 1.5 Support acceleration (g) Time (s) Fig.2 Schematic of the applied dynamic load. Thermal cycle Temperature Time (minutes) Fig.3 Schematic of the applied thermal profile.
10 318 Juan Gomez, Minghui Lin and Cemal Basaran Fig.4 Modal shapes of the first 5 modes
11 Damage Mechanics Modeling of Concurrent Thermal RESULTS AND DISCUSSION Figure 5 shows the relative displacement history at the center of the chipset for the studied frequencies. Figures 6a and 6b show the equivalent plastic strain induced by vibrations at 45Hz with two different time windows. The shown results are for the mostleft solder joint in Figure 1b. At the 1Hz and 100Hz frequencies there is no vibration induced plastic strain. Figure 7 shows the history of Von Misses equivalent stress for all the frequencies and for the thermal loading case at the same solder joint. Clearly the thermal solution alone overwhelms the Misses stresses even for the near resonance frequency of 45Hz. The equivalent plastic strain for the same loading case as in Figure 7 is shown in Figure 8. There is plastic strain at the 45Hz vibration but is almost negligible as compared to the thermal solution. In order to evaluate the validity of Miners rule we added the contributions from the independent thermal and vibration analysis and labeled this result Miners in the subsequent plots. For the 1.0Hz frequency under dynamic loads alone there is no plastic strain and the Miners solution and thermal solutions are exactly the same. Comparison with the concurrent solution at 1.0Hz is shown in Figure 9. The applied dynamic loading at this particular frequency caused no plastic strain, however it did increase the damage when applied concurrently with the thermal loading. Furthermore the concurrent loading generates larger plastic strains as compared to the thermal loading case. This result suggests that although the trend behind Miners rule is in the right direction (i.e., damage increases) the effect of the concurrent loading considerable increases damage and a linear superposition of both effects is inaccurate. Figure 10(a) and 10(b) present similar results for the 45Hz frequency for the equivalent plastic strain and Von Misses equivalent stress. In Figure 11 the case of 100Hz frequency is included in the results. Our results show that when the plastic strains due to independently applied vibrational and thermal loads are linearly added together to avoid the concurrent loading analysis the prediction underestimates the concurrent loading response. Therefore, from the computational results it can be concluded that using Miners rule leads to much smaller equivalent plastic strain and Misses stress values as compared to the concurrent application of the thermal and vibration loads.
12 320 Juan Gomez, Minghui Lin and Cemal Basaran Fig.5 1Hz, 45Hz, 100 Hz Dynamic loading only relative displacement. (a)
13 Damage Mechanics Modeling of Concurrent Thermal. 321 (b) Fig. 6 (a) 45Hz, Dynamic loading only equivalent plastic strain. (b) 45Hz, Dynamic loading only equivalent plastic strain. Fig.7 1Hz, 45Hz, 100Hz Dynamic and thermalmisses Stress
14 322 Juan Gomez, Minghui Lin and Cemal Basaran Fig.8 1Hz, 45Hz, 100Hz dynamic and thermalequivalent plastic strain. Fig.9 Equivalent plastic strain for the 1Hz Dynamic+thermal (Miners), concurrent and thermal load cases.
15 Damage Mechanics Modeling of Concurrent Thermal. 323 (a) (b) Fig.10 (a) Equivalent plastic strain for the 45Hz dynamic+thermal (Miners) and concurrent load cases. (b) Misses equivalent stress for the 45Hz dynamic+thermal (Miners) and concurrent load cases.
16 324 Juan Gomez, Minghui Lin and Cemal Basaran Fig.11 Equivalent plastic strain for the 1.0, 45.0 and 100Hz concurrent load case. 5. CONCLUSIONS AND RECOMMENDATIONS A damage mechanics coupled elastoviscoplastic constitutive model is proposed for analysis of microelectronic packaging under concurrent thermal and vibration loads. We have performed finite element analysis of electronic packaging under dynamic, thermal and concurrent (dynamic and thermal) load cases using a thermodynamics damage mechanics based rate dependent constitutive model for Pb/Sn solder alloys. The results from the simulations show that the superposition principle behind Miners rule that adds up the independent solutions from dynamic and thermal analysis to obtain the concurrent solution is correct for the boundary conditions and loading directions applied here. Yet, Miner s rule consistently underestimates the response of the system. The finite element simulations study conducted in here show that, using Miner s rule can lead to nonconservative results for certain boundary conditions and loading directions. ACKNOWLEDGMENTS This research project is supported by the United States Navy Office of Naval Research Advanced Electrical Power Systems Program, under the direction of director Terry Ericsen. REFERENCES
17 Damage Mechanics Modeling of Concurrent Thermal. 325 [1]. Kitano, B. P., Kawai, S. and Shimizu, L, Thermal Fatigue Strength Estimation of Solder Joints of Surface Mount IC Packages, Proc. 8 th Annual Int. Elec. Packaging Conf., IEPS, Dallas, Texas, pp.48, [2]. Lau, J. and Rice, J. R, Thermal Stress/ Strain Analyses of Ceramic Quad Flat Pack Packages and Interconnects, Elect. Components and Technology 40 th Conf., Vol.1, Los Vegas, Nevada, pp , [3]. Basaran, C., Chandaroy R. and Zhao, Y, Influence of Grain Size and Microstructure on Dynamic Response of Solder Joints, 98WA/EEP12, ASME Publications. [4]. Adams, P. J. Thermal Fatigue of Solder Joints in MicroElectronic Devices. M.S. thesis, Department of Mechanical Engineering, MIT, Cambridge, MA, [5]. Wilcox, J. R., Subrahmanyan, R., and Li, C. Thermal Stress Cycles and Inelastic Deformation in Solder Joints. Proc. 2 nd ASME Int. Electronic Mat. and Processing Congr., Philadelphis, PA, pp [6]. Knocht, S. and Fox. L. R. Constitutive Relation and CreepFatigue Life Model for Eutectic Tin Lead Solder. IEEE Trans Comp. Hybrids Manuf. Technol, 13 (1990) [7]. Darveaux, R. and Banerji, K. Constitutive Relations for TinBased Solder Joints. IEEE Trans. Comp. Hybrids Manuf. Technol, 15(1992) [8]. Hong, B. Z. and Burrell, L. G. Nonlinear Finite Element Simulation of Thermoviscoplastic Deformation of C4 Solder Joints in High Density Packaging Under Thermal Cycling. IEEE Trans. Components, Packaging, and Manufacturing TechnologyPart A, 18(1995) [9]. McDowell, D. L., Miller, M. P., and Brooks, D. C. A Unified CreepPlasticity Theory for Solder Alloys. Fatigue Testing of Electronic Materials, ASTM STP, 1153 (1994) [10]. Zhao, Y.. Thermomechanical Behavior of Ball Grid Array Solder Joints Under Thermal and Vibration Loading; Testing and Modeling. PhD Dissertation. University at Buffalo. The State University of New York, [11]. Basaran, C., and Tang, H., Implementation of a thermodynamic framework for damage mechanics of solder interconnect in microelectronic packaging. Proceedings of IMECE, 2002 ASME International Mechanical Engineering Congress & Exposition., New Orleans, Louisiana. [12]. Tang, H. A Thermodynamic Damage Mechanics Theory and Experimental Verification for Thermomechanical Fatigue Life Prediction of Microelectronics Solder Joints. PhD Dissertation. University at Buffalo. The State University of New York [13]. Kashyap, B., and Murty, G.. Experimental Constitutive Relations for the High Temperature Deformation of a PbSn Eutectic Alloy. Mater.Sci. and Engin, 50(1981) [14]. Gomez, J., and Basaran, C. Determination Of The Strain Gradient Plasticity Length Scale For Microelectronics Solder Alloys. Submitted to Inter. J. Plasticity. [15]. Gomez, J., and Basaran, C. Nanoindentation of Pb/Sn Solder Alloys;Experimental and Finite Element Simulation Results. Inter. J.Solids and Struc. in press [16]. Steinberg, D.S. Vibration Analysis for Electronic Equipment. 2 nd Edition., John Wiley & Sons, New York. (1988) [17]. Basaran, C., Zhao, Y., Tang, H., and Gomez, J. A Damage Mechanics Based Constitutive Model for Joints. ASME J. Electronic Packaging, 127 (2005) 17. [18]. Simo, J., and Hughes, T. Computational Inelasticity. Interdisciplinary applied mathematics. Springer [19]. Owen, D.R.J. and Hinton, E.. Finite Element in Plasticity, Pineridge Press Limited, Swansea, U.K [20]. Zhao, Y., Basaran, C., Cartwright, A., and Dishongh, T. Thermomechanical Behavior of Micron Scale Solder Joints: An Experimental Observation. J. Mech. Behavior of Mater, 10(1999) [21]. Barker, D., Vodzak, J., Dashgupta, A., and Pecht, M. Combined Vibrational and Thermal Solder Joint Fatigue. A Generalized Strain versus Life Approach. ASME J. Elec. Packaging, 2(1990) [22]. Miner, M.A. Cumulative Damage in Fatigue. ASME J. Applied Mech [23]. Lubarda, V and Benson, D.. On the numerical algorithm for isotropickinematic hardening with the ArmstrongFrederick evolution of the back stress. Comput. Methods Appl. Mech. Engrg, 191(2002)
18 326 Juan Gomez, Minghui Lin and Cemal Basaran [24]. Alfano, G., De Angelis, F., and Rosati, L. General Solution Procedures in Elasto/Viscoplasticity. Comput. Meth. Appl. Mech. Eng, 190(2001) [25]. Chaboche, J. Constitutive equations for cyclic plasticity and viscoplasticity. Inter. J. Plasticity, 3(1989) [26]. Armstrong, P. J., and Frederick, C. O. A Mathematical Representation of the Multiaxial Bauschinger Effect. CEGB Report RD/B/N [27]. Prager, W. A new method of analyzing stress and strains in workhardening plastic solids. Journal of Applied Mechanics, 23 (1956) [28]. Lemaitre, J. A course on damage mechanics.springerverlag. Germany [29]. Basaran, C., and Yan, C. A Thermodynamic Framework for Damage Mechanics of Solder Joints. Journal of Electronic Packaing, Trans. ASME, 120(1998) [30]. Basaran, C., and Nie, S. An Irreversible Thermodynamic Theory for Damage Mechanics of Solids. International Journal of Damage Mechanics, 13(2004) [31]. Gomez, J and Basaran, C. Numerical Simulation of Monotonic and Fatigue Shear Testing of Thin Layer Solder Joints Using a Damage mechanics Based Constitutive Model. Proceedings 2003 ASME Mechanics and Materials Conference, Scottsdale, Arizona. [32]. Pecht, M., Agarwal, R., Mc Cluskey, P., Dishong, T., Javadpour, S. and Mohajan, R. Electronic packaging materials and their properties. CRC press [33]. Pitarresi, M. Estimating Shock and Vibration Response in Personal Computers. Yearly Report. Department of Mechanical Engineering, State University of New York at Binghamton, December
DETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES
DETERMINATION OF TIMETEMPERATURE SHIFT FACTOR FOR LONGTERM LIFE PREDICTION OF POLYMER COMPOSITES K. Fukushima*, H. Cai**, M. Nakada*** and Y. Miyano*** * Graduate School, Kanazawa Institute of Technology
More informationApplying Anand Model to Represent the Viscoplastic Deformation Behavior of Solder Alloys
G. Z. Wang email: guozhong.wang@daimlerchyrsler.com Z. N. Cheng email: zhaonian.cheng@daimlerchrysler.com Daimler Chrysler SIM Technology, 865 Changning Road, Shanghai 200050, China K. Becker University
More informationCHAPTER 3 MODAL ANALYSIS OF A PRINTED CIRCUIT BOARD
45 CHAPTER 3 MODAL ANALYSIS OF A PRINTED CIRCUIT BOARD 3.1 INTRODUCTION This chapter describes the methodology for performing the modal analysis of a printed circuit board used in a hand held electronic
More informationTHERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE
THERMAL CRACKING RESPONE OF REINFORCED CONCRETE BEAM TO GRADIENT TEMPERATURE L. DAHMANI, M.KOUANE Abstract In this paper are illustrated the principal aspects connected with the numerical evaluation of
More informationSTUDY OF DAMRESERVOIR DYNAMIC INTERACTION USING VIBRATION TESTS ON A PHYSICAL MODEL
STUDY OF DAMRESERVOIR DYNAMIC INTERACTION USING VIBRATION TESTS ON A PHYSICAL MODEL Paulo Mendes, Instituto Superior de Engenharia de Lisboa, Portugal Sérgio Oliveira, Laboratório Nacional de Engenharia
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationLong term performance of polymers
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
More information3 Theory of small strain elastoplasticity 3.1 Analysis of stress and strain 3.1.1 Stress invariants Consider the Cauchy stress tensor σ. The characteristic equation of σ is σ 3 I 1 σ +I 2 σ I 3 δ = 0,
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More information4.3 Results... 27 4.3.1 Drained Conditions... 27 4.3.2 Undrained Conditions... 28 4.4 References... 30 4.5 Data Files... 30 5 Undrained Analysis of
Table of Contents 1 One Dimensional Compression of a Finite Layer... 3 1.1 Problem Description... 3 1.1.1 Uniform Mesh... 3 1.1.2 Graded Mesh... 5 1.2 Analytical Solution... 6 1.3 Results... 6 1.3.1 Uniform
More information3D plasticity. Write 3D equations for inelastic behavior. Georges Cailletaud, Ecole des Mines de Paris, Centre des Matériaux
3D plasticity 3D viscoplasticity 3D plasticity Perfectly plastic material Direction of plastic flow with various criteria PrandtlReuss, HenckyMises, Prager rules Write 3D equations for inelastic behavior
More informationVersion default Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 Responsable : François HAMON Clé : V6.03.161 Révision : 9783
Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 SSNP161 Biaxial tests of Summarized Kupfer: Kupfer [1] was interested to characterize the performances of the concrete under biaxial
More informationPREDICTION OF DISTORTIONS IN THROUGH HARDENING OF CYLINDRICAL STEEL WORKPIECES BY DIMENSIONAL ANALYSIS
PREDICTION OF DISTORTIONS IN THROUGH HARDENING OF CYLINDRICAL STEEL WORKPIECES BY DIMENSIONAL ANALYSIS C. Şimşir 1, T. Lübben 1, F. Hoffmann 1, H.W. Zoch 1, M. Wolff 2 1 Foundation Institute of Materials
More informationEffects of Dwell Time and Ramp Rate on LeadFree Solder Joints in FCBGA Packages
Effects of Dwell Time and Ramp Rate on LeadFree Solder Joints in FCBGA Packages Xuejun Fan, George Raiser, Vasu S. Vasudevan Intel Corporation ATD Q&R, CH5263, 5000 W. Chandler Blvd, Chandler, AZ 85226
More informationAbaqus Technology Brief. Automobile Roof Crush Analysis with Abaqus
Abaqus Technology Brief Automobile Roof Crush Analysis with Abaqus TB06RCA1 Revised: April 2007. Summary The National Highway Traffic Safety Administration (NHTSA) mandates the use of certain test procedures
More information4 The strength of the lithosphere
4 The strength of the lithosphere Constitutive equations specify the relations between stress and strain or the time derivatives of strain and thus can be used in conjunction with the equations of motion
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationEuropean Microelectronics and Packaging Symposium
European Microelectronics and Packaging Symposium Prague 16th to 18th June 2004, Czech Republic THERMAL CONDUCTIVITY OF MOLTEN LEAD FREE SOLDERS JAROMIR BILEK, JOHN ATKINSON, WILLIAM WAKEHAM University
More informationCALIBRATING MATERIAL CONSTANTS FROM EXPERIMENTAL DATA FOR LEADFREE SOLDER MATERIALS USING A PARAMETRIC OPTIMIZATION APPROACH
CALIBRATING MATERIAL CONSTANTS FROM EXPERIMENTAL DATA FOR LEADFREE SOLDER MATERIALS USING A PARAMETRIC OPTIMIZATION APPROACH Shriram Swaminathan 1, Lance Hill 2, Sandeep Urankar 3 THEME Automated Optimization
More informationINVESTIGATION OF VISCOELASTICITY AND CURE SHRINKAGE IN AN EPOXY RESIN DURING PROCESSING
TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INVESTIGATION OF VISCOELASTICITY AND CURE SHRINKAGE IN AN EPOXY RESIN DURING PROCESSING T. Shimizu *, H. Koinuma, K. Nagai Mitsubishi Heavy Industries,
More informationMeasuring intrinsic elastic modulus of Pb/Sn solder alloys
Mechanics of Materials 34 (2002) 349 362 www.elsevier.com/locate/mechmat Measuring intrinsic elastic modulus of Pb/Sn solder alloys Cemal Basaran *, Jianbin Jiang UB Electronic Packaging Laboratory, Department
More informationLifetime Model for Solder Layers
Lifetime Model for Solder Layers I. KovačevićBadstübner, A. Stupar, and J.W. Kolar ETH Zurich, Switzerland Power Electronic Systems Laboratory www.pes.ee.ethz.ch / kovacevic@lem.ee.ethz.ch 2/23 Overview
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationConstitutive Equations  Plasticity
MCEN 5023/ASEN 5012 Chapter 9 Constitutive Equations  Plasticity Fall, 2006 1 Mechanical Properties of Materials: Modulus of Elasticity Tensile strength Yield Strength Compressive strength Hardness Impact
More informationNUMERICAL ANALYSIS OF THE EFFECTS OF WIND ON BUILDING STRUCTURES
Vol. XX 2012 No. 4 28 34 J. ŠIMIČEK O. HUBOVÁ NUMERICAL ANALYSIS OF THE EFFECTS OF WIND ON BUILDING STRUCTURES Jozef ŠIMIČEK email: jozef.simicek@stuba.sk Research field: Statics and Dynamics Fluids mechanics
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationMesh Moving Techniques for FluidStructure Interactions With Large Displacements
K. Stein Department of Physics, Bethel College, St. Paul, MN 55112 T. Tezduyar Mechanical Engineering, Rice University, MS 321, Houston, TX 77005 R. Benney Natick Soldier Center, Natick, MA 01760 Mesh
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationANALYTICAL AND EXPERIMENTAL EVALUATION OF SPRING BACK EFFECTS IN A TYPICAL COLD ROLLED SHEET
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, JanFeb 2016, pp. 119130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
More informationStructural Nonlinearities
Lecture 5 Rate Independent Plasticity ANSYS Mechanical Structural Nonlinearities L51 ANSYS Mechanical Rate Independent Plasticity Chapter Overview The following will be covered in this Chapter: A. Background
More informationAccelerated Thermal Cycling and Failure Mechanisms For BGA and CSP Assemblies
Accelerated Thermal Cycling and Failure Mechanisms For BGA and CSP Assemblies Reza Ghaffarian, Ph.D. Jet Propulsion Laboratory California Institute of Technology Pasadena, California 8183542059 reza.ghaffarian@jpl.nasa.gov
More informationCharacterization of Electronic Materials Using Thermal Analysis
application Note Thermal Analysis Characterization of Electronic Materials Using Thermal Analysis Thermal analysis comprises a series of powerful techniques for the characterization of the thermal, physical,
More informationRheological Properties of Topical Formulations
Rheological Properties of Topical Formulations Hemi Nae, PhD Hydan Technologies, Inc. Key Words Complex Modulus, Creep/Recovery, Dilatant Flow, Dynamic Viscosity, Flow, Flow Curve, Flow Models, Frequency
More informationGraduate Courses in Mechanical Engineering
Graduate Courses in Mechanical Engineering MEEG 501 ADVANCED MECHANICAL ENGINEERING ANALYSIS An advanced, unified approach to the solution of mechanical engineering problems, with emphasis on the formulation
More informationDfRSoft 2Day Course Shock & Vibration: Test, Design, and Design Assurance
DfRSoft 2Day Course Shock & Vibration: Test, Design, and Design Assurance Understanding of vibration and shock stresses is important for the design of reliable products for diverse applications, ranging
More informationDYNAMICAL ANALYSIS OF SILO SURFACE CLEANING ROBOT USING FINITE ELEMENT METHOD
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, JanFeb 2016, pp. 190202, Article ID: IJMET_07_01_020 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
More informationInfrared Study of Heat Dissipation under Fatigue Crack Propagation
Infrared Study of Heat Dissipation under Fatigue Crack Propagation O. Plekhov, M. Bannikov, A. erekhina, A. Fedorova Physical foundation of strength Institute of continuous media mechanics RAS str. Ak.
More informationList of Problems Solved Introduction p. 1 Concept p. 1 Nodes p. 3 Elements p. 4 Direct Approach p. 5 Linear Spring p. 5 Heat Flow p.
Preface p. v List of Problems Solved p. xiii Introduction p. 1 Concept p. 1 Nodes p. 3 Elements p. 4 Direct Approach p. 5 Linear Spring p. 5 Heat Flow p. 6 Assembly of the Global System of Equations p.
More informationBack to Elements  Tetrahedra vs. Hexahedra
Back to Elements  Tetrahedra vs. Hexahedra Erke Wang, Thomas Nelson, Rainer Rauch CADFEM GmbH, Munich, Germany Abstract This paper presents some analytical results and some test results for different
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationChapter 2 Theory on Mechanics of Solder Materials
Chapter 2 Theory on Mechanics of Solder Materials Abstract Chapter 2 reviews the fundamental theory on mechanics of solder materials. As solder materials are subject to high operating temperatures relative
More information, YongMin Kwon 1 ) , HoYoung Son 1 ) , JeongTak Moon 2 ) ByungWook Jeong 2 ) , KyungIn Kang 2 )
Effect of Sb Addition in SnAgCu Solder Balls on the Drop Test Reliability of BGA Packages with Electroless Nickel Immersion Gold (ENIG) Surface Finish YongSung Park 1 ), YongMin Kwon 1 ), HoYoung
More informationModal Analysis of the Printed Circuit Board Based on Finite Element Method Ren Guoquan1, Li Ben1,2, Li Dongwei1, Jiao Yingqi1
2014 International Conference on Computer Science and Electronic echnology (ICCSE 2014) Modal Analysis of the Printed Circuit Board Based on Finite Element Method Ren Guoquan1, Li Ben1,2, Li Dongwei1,
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationNumerical Analysis of Transient Phenomena in Electromagnetic Forming Processes
Volume 49, Number 3, 8 359 Numerical Analysis of Transient Phenomena in Electromagnetic Forming Processes Sorin PASCA, Tiberiu VESSELENYI, Virgiliu FIRETEANU Pavel MUDURA, Tiberiu TUDORACHE, Marin TOMSE
More informationSolved with COMSOL Multiphysics 4.3
Vibrating String Introduction In the following example you compute the natural frequencies of a pretensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the
More informationTheoretical and Practical Aspects of Thermo Mechanical Reliability in Printed Circuit Boards with Copper Plated Through Holes
Theoretical and Practical Aspects of Thermo Mechanical Reliability in Printed Circuit Boards with Copper Plated Through Holes Stefan Neumann, Nina Dambrowsky, Stephen Kenny Atotech Deutschland GmbH Berlin,
More informationGuideway Joint Surface Properties of Heavy Machine Tools Based on the Theory of Similarity
Research Journal of Applied Sciences, Engineering and Technology 5(): 530536, 03 ISSN: 0407459; eissn: 0407467 Maxwell Scientific Organization, 03 Submitted: October, 0 Accepted: December 03, 0 Published:
More informationStress Relaxation Study of Paper and Plastic Film based Packaging Material
Master's Degree Thesis ISRN: BTHAMTEX2009/D02SE Stress Relaxation Study of Paper and Plastic Film based Packaging Material Rajdip Roy Lu Qi Department of Mechanical Engineering Blekinge Institute
More informationFeature Commercial codes Inhouse codes
A simple finite element solver for thermomechanical problems Keywords: Scilab, Open source software, thermoelasticity Introduction In this paper we would like to show how it is possible to develop a
More informationThree dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response
Three dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response Harrison Poon, Seid Koric, M. Fouad Ahmad National Center for
More informationFatigue Analysis and Optimization of Flexible Printed Circuits
Fatigue Analysis and Optimization of Flexible Printed Circuits Alexander Ptchelintsev Nokia Research Center P.O. Box 407, FI00045 NOKIA GROUP, Finland Email: alexander.ptchelintsev@nokia.com Abstract:
More informationDistance Learning Program
Distance Learning Program Leading To Master of Engineering or Master of Science In Mechanical Engineering Typical Course Presentation Format Program Description Clarkson University currently offers a Distance
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationCFD SIMULATION OF SDHW STORAGE TANK WITH AND WITHOUT HEATER
International Journal of Advancements in Research & Technology, Volume 1, Issue2, July2012 1 CFD SIMULATION OF SDHW STORAGE TANK WITH AND WITHOUT HEATER ABSTRACT (1) Mr. Mainak Bhaumik M.E. (Thermal Engg.)
More informationProtecting Printed Circuit Boards from Harsh Vibration Environment
Protecting Printed Circuit Boards from Harsh Vibration Environment M.I.Sakri 1, P.V.Mohanram 2 Professor, Dept. of Mechanical Engineering, BLDEA s College of Engineering & Technology, Vijayapur, India
More informationAdaptation of General Purpose CFD Code for Fusion MHD Applications*
Adaptation of General Purpose CFD Code for Fusion MHD Applications* Andrei Khodak Princeton Plasma Physics Laboratory P.O. Box 451 Princeton, NJ, 08540 USA akhodak@pppl.gov Abstract Analysis of many fusion
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationABAQUS Tutorial. 3D Modeling
Spring 2011 01/21/11 ABAQUS Tutorial 3D Modeling This exercise intends to demonstrate the steps you would follow in creating and analyzing a simple solid model using ABAQUS CAE. Introduction A solid undergoes
More informationTWODIMENSIONAL FINITE ELEMENT ANALYSIS OF FORCED CONVECTION FLOW AND HEAT TRANSFER IN A LAMINAR CHANNEL FLOW
TWODIMENSIONAL FINITE ELEMENT ANALYSIS OF FORCED CONVECTION FLOW AND HEAT TRANSFER IN A LAMINAR CHANNEL FLOW Rajesh Khatri 1, 1 M.Tech Scholar, Department of Mechanical Engineering, S.A.T.I., vidisha
More informationIntegration of a fin experiment into the undergraduate heat transfer laboratory
Integration of a fin experiment into the undergraduate heat transfer laboratory H. I. AbuMulaweh Mechanical Engineering Department, Purdue University at Fort Wayne, Fort Wayne, IN 46805, USA Email: mulaweh@engr.ipfw.edu
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationTRAVELING WAVE EFFECTS ON NONLINEAR SEISMIC BEHAVIOR OF CONCRETE GRAVITY DAMS
TRAVELING WAVE EFFECTS ON NONLINEAR SEISMIC BEHAVIOR OF CONCRETE GRAVITY DAMS H. Mirzabozorg 1, M. R. Kianoush 2 and M. Varmazyari 3 1,3 Assistant Professor and Graduate Student respectively, Department
More informationSimulation of Fatigue Damage in Solder Joints using Cohesive Zones
Simulation of Fatigue Damage in Solder Joints using Cohesive Zones Piet J.G. Schreurs, Müge Erinç, Adnan AbdulBaqi, Marc G.D. Geers Eindhoven University of Technology, Fac. Mech. Eng., Section of Materials
More informationAUTODESK SIMULATION MULTIPHYSICS 2013
AUTODESK SIMULATION MULTIPHYSICS 2013 Which Analysis to Use? FANKOM MÜHENDİSLİK 2/4/2013 AUTODESK SIMULATION MULTIPHYSICS Which Analysis to Use? Use the following guidelines to help choose the correct
More informationTypes of Elements
chapter : Modeling and Simulation 439 142 20 600 Then from the first equation, P 1 = 140(0.0714) = 9.996 kn. 280 = MPa =, psi The structure pushes on the wall with a force of 9.996 kn. (Note: we could
More informationWhen to Use Immediate Settlement in Settle 3D
When to Use Immediate Settlement in Settle 3D Most engineers agree that settlement is made up of three components: immediate, primary consolidation and secondary consolidation (or creep). Most engineers
More informationCharacterization and Simulation of Processes
Characterization and Simulation of Processes * M. Engelhardt 1, H. von Senden genannt Haverkamp 1, Y.Kiliclar 2, M. Bormann 1, F.W. Bach 1, S. Reese 2 1 Institute of Materials Science, Leibniz University
More informationNumerical Analysis of the Resin Transfer Molding Process via PAM RTM Software
Defect and Diffusion Forum Vol 365 (2015) pp 8893 (2015) Trans Tech Publications, Switzerland doi:10.4028/www.scientific.net/ddf.365.88 Numerical Analysis of the Resin Transfer Molding Process via PAM
More informationMASTER DEGREE PROJECT
MASTER DEGREE PROJECT Finite Element Analysis of a Washing Machine Cylinder Thesis in Applied Mechanics one year Master Degree Program Performed : Spring term, 2010 Level Author Supervisor s Examiner :
More informationProgramming the Finite Element Method
Programming the Finite Element Method FOURTH EDITION I. M. Smith University of Manchester, UK D. V. Griffiths Colorado School of Mines, USA John Wiley & Sons, Ltd Contents Preface Acknowledgement xv xvii
More informationRESILIENT MODULUS: WHAT, WHY, AND HOW?
RESILIENT MODULUS: WHAT, WHY, AND HOW? Shane Buchanan, Vulcan Materials Company, 08/1/07 Resilient modulus (M r ) continues to be a key design parameter for pavement systems. Accurate knowledge of the
More informationThermal Fatigue Assessment of LeadFree Solder Joints
Thermal Fatigue Assessment of LeadFree Solder Joints Qiang YU and Masaki SHIRATORI Department of Mechanical Engineering and Materials Science Yokohama National University Tokiwadai 795, Hodogayaku,
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationAnalysis of Mobile Phone Reliability Based on Active Disassembly Using Smart Materials *
Journal of Surface Engineered Materials and Advanced Technology, 2011, 1, 8087 doi:10.4236/jsemat.2011.12012 Published Online July 2011 (http://www.scirp.org/journal/jsemat) Analysis of Mobile Phone Reliability
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationLecture 18 Strain Hardening And Recrystallization
138 Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing
More informationThe stored energy of cold work: Predictions from discrete dislocation plasticity
Acta Materialia 53 (2005) 4765 4779 www.actamatjournals.com The stored energy of cold work: Predictions from discrete dislocation plasticity A.A. Benzerga a, *, Y. Bréchet b, A. Needleman c, E. Van der
More informationPREDICTION OF MACHINE TOOL SPINDLE S DYNAMICS BASED ON A THERMOMECHANICAL MODEL
PREDICTION OF MACHINE TOOL SPINDLE S DYNAMICS BASED ON A THERMOMECHANICAL MODEL P. Kolar, T. Holkup Research Center for Manufacturing Technology, Faculty of Mechanical Engineering, CTU in Prague, Czech
More informationMASTER OF SCIENCE IN MECHANICAL ENGINEERING
MASTER OF SCIENCE IN MECHANICAL ENGINEERING Introduction There are over 22 schools in Mindanao that offer Bachelor of Science in Mechanical Engineering and majority of their faculty members do not have
More informationChapter 1. Governing Equations of Fluid Flow and Heat Transfer
Chapter 1 Governing Equations of Fluid Flow and Heat Transfer Following fundamental laws can be used to derive governing differential equations that are solved in a Computational Fluid Dynamics (CFD) study
More informationLaminar Flow and Heat Transfer of HerschelBulkley Fluids in a Rectangular Duct; FiniteElement Analysis
Tamkang Journal of Science and Engineering, Vol. 12, No. 1, pp. 99 107 (2009) 99 Laminar Flow and Heat Transfer of HerschelBulkley Fluids in a Rectangular Duct; FiniteElement Analysis M. E. SayedAhmed
More informationNUMERICAL MODELLING OF PIEZOCONE PENETRATION IN CLAY
NUMERICAL MODELLING OF PIEZOCONE PENETRATION IN CLAY Ilaria Giusti University of Pisa ilaria.giusti@for.unipi.it Andrew J. Whittle Massachusetts Institute of Technology ajwhittl@mit.edu Abstract This paper
More informationDYNAMIC ANALYSIS OF THICK PLATES SUBJECTED TO EARTQUAKE
DYNAMIC ANALYSIS OF THICK PLATES SUBJECTED TO EARTQUAKE ÖZDEMİR Y. I, AYVAZ Y. Posta Adresi: Department of Civil Engineering, Karadeniz Technical University, 68 Trabzon, TURKEY Eposta: yaprakozdemir@hotmail.com
More informationBenchmark Tests on ANSYS Parallel Processing Technology
Benchmark Tests on ANSYS Parallel Processing Technology Kentaro Suzuki ANSYS JAPAN LTD. Abstract It is extremely important for manufacturing industries to reduce their design process period in order to
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationNumerical Simulation of CPT Tip Resistance in Layered Soil
Numerical Simulation of CPT Tip Resistance in Layered Soil M.M. Ahmadi, Assistant Professor, mmahmadi@sharif.edu Dept. of Civil Engineering, Sharif University of Technology, Tehran, Iran Abstract The paper
More informationFEM simulation of the size and constraining effect in lead free solder joints
Applied and Computational Mechanics 6 (2012) 17 24 FEM simulation of the size and constraining effect in lead free solder joints M. Lederer a,, G. Khatibi a, B. Weiss a a Faculty of Physics, University
More informationNUMERICAL AND EXPERIMENTAL ANALYSIS OF ICE MELTING IN WATER
0HFiQLFD&RPSXWDFLRQDO9RO;;,SS± 5,GHOVRKQ9(RQ]RJQLDQG$&DUGRQD(GV DQWD)H±3DUDQi$UJHQWLQD2FWREHU NUMERICAL AND EXPERIMENTAL ANALYSIS OF ICE MELTING IN WATER Cristian A. Peña, Marcela A. Cruchaga and Diego
More informationValidation of Virtual Life Management for Electronic Solder Materials. VEXTEC Corporation 5123 Virginia Way, C21, Brentwood, TN 37027
Validation of Virtual Life Management for Electronic Solder Materials VEXTEC Corporation 53 Virginia Way, C, Brentwood, TN 377 Abstract: Electronic failures can result in immediate system shutdown with
More informationParticular analysis of vibration energy transmission in connections of thin plates
Particular analysis of vibration energy transmission in connections of thin plates J. Cieslik AGHUST University of Science and Technology, Al. Mickiewicza 30, 30059 Krakow, Poland cieslik@agh.edu.pl
More informationTesting and appraisal of Lucobit polymer effect as an additive on asphalt mixture performance
Abstract Testing and appraisal of polymer effect as an additive on asphalt mixture performance Hamid Sabbagh mollahosseini*,golazin Yadollahi**, Ershad Amoosoltani*** *, ***Executive of Engineering and
More informationDAMAGE AND FATIGUE Continuum Damage Mechanics modeling for fatigue of materials and structures. Rodrigue Desmorat
DAMAGE AND FATIGUE Continuum Damage Mechanics modeling for fatigue of materials and structures Rodrigue Desmorat LMT Cachan ENS Cachan, 61 av. du Pt Wilson 94235 Cachan Cedex desmorat@lmt.enscachan.fr
More informationDEVELOPMENT OF HIGH SPEED RESPONSE LAMINAR FLOW METER FOR AIR CONDITIONING
DEVELOPMENT OF HIGH SPEED RESPONSE LAMINAR FLOW METER FOR AIR CONDITIONING Toshiharu Kagawa 1, Yukako Saisu 2, Riki Nishimura 3 and Chongho Youn 4 ABSTRACT In this paper, we developed a new laminar flow
More information